单质电阻率列表

本文汇总元素单质的电阻率。

## 电阻率列表

T｜80 K (−193 °C)｜273 K (0 °C)｜293 K (20 °C)｜298 K (25 °C)｜300 K (27 °C)｜500 K (227 °C)

3 Li 锂

use｜10.0 nΩm｜85.3 nΩm｜92.8 nΩm｜94.7 nΩm｜95.5 nΩm

CRC (10−8 Ωm)｜1.00｜8.53｜9.28｜9.47｜9.55

LNG (10−8 Ωm)｜9.28

WEL (10−8 Ωm)｜(293 K–298 K) 9.4

4 Be 铍

use｜0.75 nΩm｜30.2 nΩm｜35.6 nΩm｜37.0 nΩm｜37.6 nΩm｜99 nΩm

CRC (10−8 Ωm)｜0.075｜3.02｜3.56｜3.70｜3.76｜9.9

LNG (10−8 Ωm)｜3.56

WEL (10−8 Ωm)｜(293 K–298 K) 4

5 B 硼

use｜1.5×104 Ωm

LNG (10−8 Ωm)｜1.5×1012

WEL (10−8 Ωm)｜(293 K–298 K) > 1012

6 C 碳 (金刚石)

use

LNG (10−8 Ωm)｜0.8 sic

6 C 碳 (石墨)

use

LNG (10−8 Ωm)｜1375

WEL (10−8 Ωm)｜(293 K–298 K) 约1000 – direction dependent

11 Na 钠

use｜8.0 nΩm｜43.3 nΩm｜47.7 nΩm｜48.8 nΩm｜49.3 nΩm

CRC (10−8 Ωm)｜0.80｜4.33｜4.77｜4.88｜4.93

LNG (10−8 Ωm)｜4.77

WEL (10−8 Ωm)｜(293 K–298 K) 4.7

12 Mg 镁

use｜5.57 nΩm｜40.5 nΩm｜43.9 nΩm｜44.8 nΩm｜45.1 nΩm｜78.6 nΩm

CRC (10−8 Ωm)｜0.557｜4.05｜4.39｜4.48｜4.51｜7.86

LNG (10−8 Ωm)｜4.39

WEL (10−8 Ωm)｜(293 K–298 K) 4.4

13 Al 铝

use｜2.45 nΩm｜24.17 nΩm｜26.50 nΩm｜27.09 nΩm｜27.33 nΩm｜49.9 nΩm

CRC (10−8 Ωm)｜0.245｜2.417｜2.650｜2.709｜2.733｜4.99

LNG (10−8 Ωm)｜2.6548

WEL (10−8 Ωm)｜(293 K–298 K) 2.65

14 Si 硅use

LNG (10−8 Ωm)｜105

WEL (10−8 Ωm)｜(293 K–298 K) 约100000

15 P 磷use

LNG (10−8 Ωm)｜(white) 10 sic

WEL (10−8 Ωm)｜(293 K–298 K) 10

16 S 硫

use｜(无定形) 2×1015 Ωm

LNG (10−8 Ωm)｜(无定形) 2×1023

WEL (10−8 Ωm)｜(293 K–298 K) > 1023

17 Cl 氯

use｜> 10 Ωm

LNG (10−8 Ωm)｜>109

WEL (10−8 Ωm)｜(293 K–298 K) > 1010

19 K 钾

use｜13.4 nΩm｜64.9 nΩm｜72.0 nΩm｜73.9 nΩm｜74.7 nΩm

CRC (10−8 Ωm)｜1.34｜6.49｜7.20｜7.39｜7.47

LNG (10−8 Ωm)｜7.2

WEL (10−8 Ωm)｜(293 K–298 K) 7

20 Ca 钙

use｜6.5 nΩm｜31.1 nΩm｜33.6 nΩm｜34.2 nΩm｜34.5 nΩm｜60. nΩm

CRC (10−8 Ωm)｜0.65｜3.11｜3.36｜3.42｜3.45｜6.0

LNG (10−8 Ωm)｜3.36

WEL (10−8 Ωm)｜(293 K–298 K) 3.4

21 Sc 钪

use｜(室温) (α，多晶) 562 nΩm（计算）

CRC (10−8 Ωm)｜(290 K–300 K) 56.2

CR2 (10−8 Ωm)｜(室温) (α，无定形) 70.9

CR2 (10−8 Ωm)｜(室温) (α，晶体) 26.9

CR2 (10−8 Ωm)｜(室温) (α，多晶) 56.2（据单晶计算）

LNG (10−8 Ωm)｜56.2

WEL (10−8 Ωm)｜(293 K–298 K) 55

22 Ti 钛

use｜0.39 µΩm｜0.420 µΩm

CRC (10−8 Ωm)｜39

LNG (10−8 Ωm)｜42.0

WEL (10−8 Ωm)｜(293 K–298 K) 40

23 V 钒

use｜24.1 nΩm｜181 nΩm｜197 nΩm｜201 nΩm｜202 nΩm｜348 nΩm

CRC (10−8 Ωm)｜2.41｜18.1｜19.7｜20.1｜20.2｜34.8

LNG (10−8 Ωm)｜19.7

WEL (10−8 Ωm)｜(293 K–298 K) 20

24 Cr 铬

use｜118 nΩm｜125 nΩm｜126 nΩm｜127 nΩm｜201 nΩm

CRC (10−8 Ωm)｜11.8｜12.5｜12.6｜12.7｜20.1

LNG (10−8 Ωm)｜12.5

WEL (10−8 Ωm)｜(293 K–298 K) 12.7

25 Mn 锰

use｜1.32 µΩm｜1.43 µΩm｜1.44 µΩm｜1.44 µΩm｜1.44 µΩm｜1.49 µΩm

CRC (10−8 Ωm)｜132｜143｜144｜144｜144｜149

LNG (10−8 Ωm)｜144

WEL (10−8 Ωm)｜(293 K–298 K) 160

26 Fe 铁

use｜6.93 nΩm｜85.7 nΩm｜96.1 nΩm｜98.7 nΩm｜99.8 nΩm｜237 nΩm

CRC (10−8 Ωm)｜0.693｜8.57｜9.61｜9.87｜9.98｜23.7

LNG (10−8 Ωm)｜9.61

WEL (10−8 Ωm)｜(293 K–298 K) 9.7

27 Co 钴

use｜56 nΩm｜62.4 nΩm

CRC (10−8 Ωm)｜5.6

LNG (10−8 Ωm)｜6.24

WEL (10−8 Ωm)｜(293 K–298 K) 6

28 Ni 镍

use｜5.45 nΩm｜61.6 nΩm｜69.3 nΩm｜71.2 nΩm｜72.0 nΩm｜177 nΩm

CRC (10−8 Ωm)｜0.545｜6.16｜6.93｜7.12｜7.20｜17.7

LNG (10−8 Ωm)｜6.93

WEL (10−8 Ωm)｜(293 K–298 K) 7

29 Cu 铜

use｜2.15 nΩm｜15.43 nΩm｜16.78 nΩm｜17.12 nΩm｜17.25 nΩm｜30.90 nΩm

CRC (10−8 Ωm)｜0.215｜1.543｜1.678｜1.712｜1.725｜3.090

LNG (10−8 Ωm)｜1.678

WEL (10−8 Ωm)｜(293 K–298 K) 1.7

30 Zn 锌

use｜11.5 nΩm｜54.6 nΩm｜59.0 nΩm｜60.1 nΩm｜60.6 nΩm｜108.2 nΩm

CRC (10−8 Ωm)｜1.15｜5.46｜5.90｜6.01｜6.06｜10.82

LNG (10−8 Ωm)｜5.9

WEL (10−8 Ωm)｜(293 K–298 K) 5.9

31 Ga 镓use

CRC (10−8 Ωm)｜13.6

LNG (10−8 Ωm)｜(30 °C) 25.795

WEL (10−8 Ωm)｜(293 K–298 K) 14

32 Ge 锗use

LNG (10−8 Ωm)｜53000

WEL (10−8 Ωm)｜(293 K–298 K) 约50000

33 As 砷

use｜333 nΩm

LNG (10−8 Ωm)｜33.3

WEL (10−8 Ωm)｜(293 K–298 K) 30

34 Se 硒use

LNG (10−8 Ωm)｜(无定形) 1.2 sic

WEL (10−8 Ωm)｜(293 K–298 K) high

35 Br 溴

use｜7.8×1010 Ωm

LNG (10−8 Ωm)｜7.8×1018

WEL (10−8 Ωm)｜(293 K–298 K) > 1018

37 Rb 铷

use｜26.5 nΩm｜115 nΩm｜128 nΩm｜131 nΩm｜133 nΩm

CRC (10−8 Ωm)｜2.65｜11.5｜12.8｜13.1｜13.3

LNG (10−8 Ωm)｜12.8

WEL (10−8 Ωm)｜(293 K–298 K) 12

38 Sr 锶

use｜36.4 nΩm｜123 nΩm｜132 nΩm｜134 nΩm｜135 nΩm｜222 nΩm

CRC (10−8 Ωm)｜3.64｜12.3｜13.2｜13.4｜13.5｜22.2

LNG (10−8 Ωm)｜13.2

WEL (10−8 Ωm)｜(293 K–298 K) 13

39 Y 钇

use｜(室温) (α，多晶) 596 nΩm

CRC (10−8 Ωm)｜(290 K–300 K) 59.6

CR2 (10−8 Ωm)｜(室温) (α，无定形) 72.5

CR2 (10−8 Ωm)｜(室温) (α，晶体) 35.5

CR2 (10−8 Ωm)｜(室温) (α，多晶) 59.6

LNG (10−8 Ωm)｜59.6

WEL (10−8 Ωm)｜(293 K–298 K) 56

40 Zr 锆

use｜66.4 nΩm｜388 nΩm｜421 nΩm｜429 nΩm｜433 nΩm｜765 nΩm

CRC (10−8 Ωm)｜6.64｜38.8｜42.1｜42.9｜43.3｜76.5

LNG (10−8 Ωm)｜42.1

WEL (10−8 Ωm)｜(293 K–298 K) 42

41 Nb 铌

use｜152 nΩm

CRC (10−8 Ωm)｜15.2

LNG (10−8 Ωm)｜15.2

WEL (10−8 Ωm)｜(293 K–298 K) 15

42 Mo 钼

use｜4.82 nΩm｜48.5 nΩm｜53.4 nΩm｜54.7 nΩm｜55.2 nΩm｜106 nΩm

CRC (10−8 Ωm)｜0.482｜4.85｜5.34｜5.47｜5.52｜10.6

LNG (10−8 Ωm)｜5.34

WEL (10−8 Ωm)｜(293 K–298 K) 5

43 Tc 锝use

LNG (10−8 Ωm)｜(100 °C) 22.6

WEL (10−8 Ωm)｜(293 K–298 K) 20

44 Ru 钌

use｜71 nΩm

CRC (10−8 Ωm)｜7.1

LNG (10−8 Ωm)｜7.1

WEL (10−8 Ωm)｜(293 K–298 K) 7.1

45 Rh 铑

use｜43.3 nΩm

CRC (10−8 Ωm)｜4.3

LNG (10−8 Ωm)｜4.33

WEL (10−8 Ωm)｜(293 K–298 K) 4.3

46 Pd 钯

use｜17.5 nΩm｜97.8 nΩm｜105.4 nΩm｜107.3 nΩm｜108.0 nΩm｜179.4 nΩm

CRC (10−8 Ωm)｜1.75｜9.78｜10.54｜10.73｜10.80｜17.94

LNG (10−8 Ωm)｜10.54

WEL (10−8 Ωm)｜(293 K–298 K) 10

47 Ag 银

use｜2.89 nΩm｜14.67 nΩm｜15.87 nΩm｜16.17 nΩm｜16.29 nΩm｜28.7 nΩm

CRC (10−8 Ωm)｜0.289｜1.467｜1.587｜1.617｜1.629｜2.87

LNG (10−8 Ωm)｜1.587

WEL (10−8 Ωm)｜(293 K–298 K) 1.6

48 Cd 镉

use｜68 nΩm

use｜(22 °C) 72.7 nΩm

CRC (10−8 Ωm)｜6.8

LNG (10−8 Ωm)｜(22 °C) 7.27

WEL (10−8 Ωm)｜(293 K–298 K) 7

49 In 铟

use｜0.080 µΩm｜83.7 nΩm

CRC (10−8 Ωm)｜8.0

LNG (10−8 Ωm)｜8.37

WEL (10−8 Ωm)｜(293 K–298 K) 8

50 Sn 锡

use｜115 nΩm

CRC (10−8 Ωm)｜11.5

LNG (10−8 Ωm)｜11.5

WEL (10−8 Ωm)｜(293 K–298 K) 11

51 Sb 锑

use｜0.39 µΩm｜417 nΩm

CRC (10−8 Ωm)｜39

LNG (10−8 Ωm)｜41.7

WEL (10−8 Ωm)｜(293 K–298 K) 40

52 Te 碲use

LNG (10−8 Ωm)｜(5.8–33)×10³

WEL (10−8 Ωm)｜(293 K–298 K) 约10000

53 I 碘

use｜1.3×107 Ωm

LNG (10−8 Ωm)｜1.3×1015

WEL (10−8 Ωm)｜(293 K–298 K) > 1015

55 Cs 铯

use｜41.6 nΩm｜187 nΩm｜205 nΩm｜208 nΩm｜210 nΩm

CRC (10−8 Ωm)｜4.16｜18.7｜20.5｜20.8｜21.0

LNG (10−8 Ωm)｜20.5

WEL (10−8 Ωm)｜(293 K–298 K) 20

56 Ba 钡

use｜68.3 nΩm｜302 nΩm｜332 nΩm｜0.340 µΩm｜343 nΩm｜724 nΩm

CRC (10−8 Ωm)｜6.83｜30.2｜33.2｜34.0｜34.3｜72.4

LNG (10−8 Ωm)｜33.2

WEL (10−8 Ωm)｜(293 K–298 K) 35

57 La 镧

use｜(室温) (α，多晶) 615 nΩm

CRC (10−8 Ωm)｜(290 K–300 K) 61.5

CR2 (10−8 Ωm)｜(室温) (α，多晶) 61.5

LNG (10−8 Ωm)｜61.5

WEL (10−8 Ωm)｜(293 K–298 K) 61

58 Ce 铈 (β，hex)

use｜(室温) (β，多晶) 828 nΩm

CRC (10−8 Ωm)｜(β，hex) (290 K–300 K) 82.8

CR2 (10−8 Ωm)｜(室温) (β，多晶) 82.8

LNG (10−8 Ωm)｜(β，hex) 82.8

58 Ce 铈 (γ，cubic)

use｜(室温) (γ，多晶) 744 nΩm

CRC (10−8 Ωm)｜74.4

CR2 (10−8 Ωm)｜(室温) (γ，多晶) 74.4

WEL (10−8 Ωm)｜(293 K–298 K) 74

59 Pr 镨

use｜(室温) (α，多晶) 0.700 µΩm

CRC (10−8 Ωm)｜(290 K–300 K) 70.0

CR2 (10−8 Ωm)｜(室温) (α，多晶) 70.0

LNG (10−8 Ωm)｜70.0

WEL (10−8 Ωm)｜(293 K–298 K) 70

60 Nd 钕

use｜(室温) (α，多晶) 643 nΩm

CRC (10−8 Ωm)｜(290 K–300 K) 64.3

CR2 (10−8 Ωm)｜(室温) (α，多晶) 64.3

LNG (10−8 Ωm)｜64.3

WEL (10−8 Ωm)｜(293 K–298 K) 64

61 Pm 钷

use｜(室温) 0.75 µΩm（估）

CRC (10−8 Ωm)｜(290 K–300 K) 75（估）

CR2 (10−8 Ωm)｜(室温) (α，多晶) 75（估）

LNG (10−8 Ωm)｜64.0

WEL (10−8 Ωm)｜(293 K–298 K) 75

62 Sm 钐

use｜(室温) (α，多晶) 0.940 µΩm

CRC (10−8 Ωm)｜(290 K–300 K) 94.0

CR2 (10−8 Ωm)｜(室温) (α，多晶) 94.0

LNG (10−8 Ωm)｜94.0

WEL (10−8 Ωm)｜(293 K–298 K) 94

63 Eu 铕

use｜(室温) (多晶) 0.900 µΩm

CRC (10−8 Ωm)｜(290 K–300 K) 90.0

CR2 (10−8 Ωm)｜(室温) (多晶) 90.0

LNG (10−8 Ωm)｜90.0

WEL (10−8 Ωm)｜(293 K–298 K) 90

64 Gd 钆

use｜(室温) (α，多晶) 1.310 µΩm

CRC (10−8 Ωm)｜(290 K–300 K) 131

CR2 (10−8 Ωm)｜(室温) (α，无定形) 135.1

CR2 (10−8 Ωm)｜(室温) (α，晶体) 121.7

CR2 (10−8 Ωm)｜(室温) (α，多晶) 131.0

LNG (10−8 Ωm)｜131

WEL (10−8 Ωm)｜(293 K–298 K) 130

65 Tb 铽

use｜(室温) (α，多晶) 1.150 µΩm

CRC (10−8 Ωm)｜(290 K–300 K) 115

CR2 (10−8 Ωm)｜(室温) (α，无定形) 123.5

CR2 (10−8 Ωm)｜(室温) (α，晶体) 101.5

CR2 (10−8 Ωm)｜(室温) (α，多晶) 115.0

LNG (10−8 Ωm)｜115

WEL (10−8 Ωm)｜(293 K–298 K) 120

66 Dy 镝

use｜(室温) (α，多晶) 926 nΩm

CRC (10−8 Ωm)｜(290 K–300 K) 92.6

CR2 (10−8 Ωm)｜(室温) (α，无定形) 111.0

CR2 (10−8 Ωm)｜(室温) (α，晶体) 76.6

CR2 (10−8 Ωm)｜(室温) (α，多晶) 92.6

LNG (10−8 Ωm)｜92.6

WEL (10−8 Ωm)｜(293 K–298 K) 91

67 Ho 钬

use｜(室温) (多晶) 814 nΩm

CRC (10−8 Ωm)｜(290 K–300 K) 81.4

CR2 (10−8 Ωm)｜(室温) (无定形) 101.5

CR2 (10−8 Ωm)｜(室温) (晶体) 60.5

CR2 (10−8 Ωm)｜(室温) (多晶) 81.4

LNG (10−8 Ωm)｜81.4

WEL (10−8 Ωm)｜(293 K–298 K) 94

68 Er 铒

use｜(室温) (多晶) 0.860 µΩm

CRC (10−8 Ωm)｜(290 K–300 K) 86.0

CR2 (10−8 Ωm)｜(室温) (无定形) 94.5

CR2 (10−8 Ωm)｜(室温) (晶体) 60.3

CR2 (10−8 Ωm)｜(室温) (多晶) 86.0

LNG (10−8 Ωm)｜86.0

WEL (10−8 Ωm)｜(293 K–298 K) 86

69 Tm 铥

use｜(室温) (多晶) 676 nΩm

CRC (10−8 Ωm)｜(290 K–300 K) 67.6

CR2 (10−8 Ωm)｜(室温) (无定形) 88.0

CR2 (10−8 Ωm)｜(室温) (晶体) 47.2

CR2 (10−8 Ωm)｜(室温) (多晶) 67.6

LNG (10−8 Ωm)｜67.6

WEL (10−8 Ωm)｜(293 K–298 K) 70

70 Yb 镱

use｜(室温) (β，多晶) 0.250 µΩm

CRC (10−8 Ωm)｜(290 K–300 K) 25.0

CR2 (10−8 Ωm)｜(室温) (β，多晶) 25.0

LNG (10−8 Ωm)｜25

WEL (10−8 Ωm)｜(293 K–298 K) 28

71 Lu 镥

use｜(室温) (多晶) 582 nΩm

CRC (10−8 Ωm)｜(290 K–300 K) 58.2

CR2 (10−8 Ωm)｜(室温) (无定形) 76.6

CR2 (10−8 Ωm)｜(室温) (晶体) 34.7

CR2 (10−8 Ωm)｜(室温) (多晶) 58.2

LNG (10−8 Ωm)｜58.2

WEL (10−8 Ωm)｜(293 K–298 K) 56

72 Hf 铪

use｜67.5 nΩm｜304 nΩm｜331 nΩm｜337 nΩm｜0.340 µΩm｜631 nΩm

CRC (10−8 Ωm)｜6.75｜30.4｜33.1｜33.7｜34.0｜63.1

LNG (10−8 Ωm)｜33.1

WEL (10−8 Ωm)｜(293 K–298 K) 30

73 Ta 钽

use｜26.2 nΩm｜122 nΩm｜131 nΩm｜134 nΩm｜135 nΩm｜229 nΩm

CRC (10−8 Ωm)｜2.62｜12.2｜13.1｜13.4｜13.5｜22.9

LNG (10−8 Ωm)｜13.5

WEL (10−8 Ωm)｜(293 K–298 K) 13

74 W 钨

use｜6.06 nΩm｜48.2 nΩm｜52.8 nΩm｜53.9 nΩm｜54.4 nΩm｜103 nΩm

CRC (10−8 Ωm)｜0.606｜4.82｜5.28｜5.39｜5.44｜10.3

LNG (10−8 Ωm)｜5.28

WEL (10−8 Ωm)｜(293 K–298 K) 5

75 Re 铼

use｜172 nΩm｜193 nΩm

CRC (10−8 Ωm)｜17.2

LNG (10−8 Ωm)｜19.3

WEL (10−8 Ωm)｜(293 K–298 K) 18

76 Os 锇

use｜81.2 nΩm

CRC (10−8 Ωm)｜8.1

LNG (10−8 Ωm)｜8.12

WEL (10−8 Ωm)｜(293 K–298 K) 8.1

77 Ir 铱

use｜47 nΩm｜47.1 nΩm

CRC (10−8 Ωm)｜4.7

LNG (10−8 Ωm)｜4.71

WEL (10−8 Ωm)｜(293 K–298 K) 4.7

78 Pt 铂

use｜19.22 nΩm｜96 nΩm｜105 nΩm｜107 nΩm｜108 nΩm｜183 nΩm

CRC (10−8 Ωm)｜1.922｜9.6｜10.5｜10.7｜10.8｜18.3

LNG (10−8 Ωm)｜10.6

WEL (10−8 Ωm)｜(293 K–298 K) 10.6

79 Au 金

use｜4.81 nΩm｜20.51 nΩm｜22.14 nΩm｜22.55 nΩm｜22.71 nΩm｜39.7 nΩm

CRC (10−8 Ωm)｜0.481｜2.051｜2.214｜2.255｜2.271｜3.97

LNG (10−8 Ωm)｜2.214

WEL (10−8 Ωm)｜(293 K–298 K) 2.2

80 Hg 汞

use｜961 nΩm

CRC (10−8 Ωm)｜96.1

LNG (10−8 Ωm)｜(固) 21

LNG (10−8 Ωm)｜(液) 95.8

WEL (10−8 Ωm)｜(293 K–298 K) 96

81 Tl 铊

use｜0.15 µΩm｜0.18 µΩm

CRC (10−8 Ωm)｜15

LNG (10−8 Ωm)｜18

WEL (10−8 Ωm)｜(293 K–298 K) 15

82 Pb 铅

use｜49 nΩm｜192 nΩm｜208 nΩm｜211 nΩm｜213 nΩm｜383 nΩm

CRC (10−8 Ωm)｜4.9｜19.2｜20.8｜21.1｜21.3｜38.3

LNG (10−8 Ωm)｜20.8

WEL (10−8 Ωm)｜(293 K–298 K) 21

83 Bi 铋

use｜1.07 µΩm｜1.29 µΩm

CRC (10−8 Ωm)｜107

LNG (10−8 Ωm)｜129

WEL (10−8 Ωm)｜(293 K–298 K) 130

84 Po 钋

use｜(α) 0.40 µΩm

CRC (10−8 Ωm)｜40

LNG (10−8 Ωm)｜(α) 40.0

WEL (10−8 Ωm)｜(293 K–298 K) 43

88 Ra 镭

use｜1 µΩm

LNG (10−8 Ωm)｜100

WEL (10−8 Ωm)｜(293 K–298 K) 100

90 Th 钍

use｜147 nΩm

use｜(22 °C) 15.4

CRC (10−8 Ωm)｜14.7

LNG (10−8 Ωm)｜(22 °C) 15.4

WEL (10−8 Ωm)｜(293 K–298 K) 15

91 Pa 镤

use｜177 nΩm

use｜(22 °C) 19.1

CRC (10−8 Ωm)｜17.7

LNG (10−8 Ωm)｜(22 °C) 19.1

WEL (10−8 Ωm)｜(293 K–298 K) 18

92 U 铀

use｜0.280 µΩm

CRC (10−8 Ωm)｜28

LNG (10−8 Ωm)｜28.0

WEL (10−8 Ωm)｜(293 K–298 K) 28

93 Np 镎

use｜(22 °C) 1.220 µΩm

LNG (10−8 Ωm)｜(22 °C) 122.0

WEL (10−8 Ωm)｜(293 K–298 K) 120

94 Pu 钚

use｜1.460 µΩm

LNG (10−8 Ωm)｜146.0

WEL (10−8 Ωm)｜(293 K–298 K) 150

95 Am 镅

use｜(室温) 689 nΩm

96 Cm 锔

use｜(室温) 1250 nΩm

T｜80 K (−193 °C)｜273 K (0 °C)｜293 K (20 °C)｜298 K (25 °C)｜300 K (27 °C)｜500 K (227 °C)